Source: https://www.scribd.com/document/176827379/SportMaster-Concrete-Tennis-Court-Surface-Color-Coating-System-Guide-SpecificationCP
Timestamp: 2017-04-24 02:40:38
Document Index: 361844196

Matched Legal Cases: ['ART 1', 'ART 2', 'ART 3', 'arts3366', 'arts3369', 'arts3369', 'arts3369', 'arts3366']

SportMaster Concrete Tennis Court Surface Color Coating System - Guide SpecificationCP | Acrylic Paint | Concrete
ScribdBrowseInterestsPolitics & Current AffairsCareer & MoneyPersonal GrowthFictionHealth & FitnessLifestyleEntertainmentBiographies & HistoryScience & TechBrowse byBooksAudiobooksNews & MagazinesSheet MusicBrowse allUploadSign inJoinSportMaster Concrete Tennis Court Surface Color Coating System - Guide SpecificationCPUploaded by insane88Acrylic PaintConcreteColorPaintCoating0.0 (0)DownloadEmbedDescription: tennis floorView Moretennis floorCopyright: Attribution Non-Commercial (BY-NC)List price: $0.00Download as PDF, TXT or read online from ScribdFlag for inappropriate contentSportMaster Sport Surfaces PO Box 2277 2520 South Campbell Street Sandusky, Ohio 44870 Toll Free 800-326-1994 Fax 877-825-9226 Website www.sportmaster.net E-mail info@sportmaster.net Product Guide Specification
Specifier Notes: This product guide specification is written according to the Construction Specifications Institute (CSI) 3-Part Format, including MasterFormat, SectionFormat, and PageFormat, as described in The Project Resource Manual—CSI Manual of Practice, Fifth Edition. This section must be carefully reviewed and edited by the Architect to meet the requirements of the project and local building code. Coordinate this section with other specification sections and the Drawings. Delete all “Specifier Notes” after editing this section. Section numbers are from MasterFormat 1995 Edition, with section numbers from MasterFormat 2004 Edition in parentheses. Delete version not required.
SECTION 02790 (32 18 23.53) CONCRETE TENNIS COURT SURFACE COLOR COATING SYSTEM
Specifier Notes: This section covers SportMaster Sport Surfaces “SportMaster” concrete tennis court surface color coating system. Consult SportMaster Sport Surfaces for assistance in editing this section for the specific application.
PART 1 1.1 A. 1.2
SECTION INCLUDES Concrete tennis court surface color coating system. RELATED REQUIREMENTS
Specifier Notes: Edit the following list of related sections as required. Delete related sections not required. List other sections with work directly related to this section. A. Section 03300 (03 30 00) – Cast-in-Place Concrete.
SportMaster Concrete Tennis Court Surface Color Coating System
02790 (32 18 23.53) - 1
but is merely a listing of those used. A. Delete submittals not required. Test Reports: Submit independent test results for solar reflectance index. 1. including project name. type and quantity of color coating system applied. location.
G. Manufacturer’s Certification: Submit manufacturer’s certification that materials comply with specified requirements and are suitable for intended application. including surface and crack preparation and application instructions.3
Section 03400 (03 40 00) – Precast Concrete.
C. American Sports Builders Association (ASBA).
1.5 A. QUALITY ASSURANCE Manufacturer’s Qualifications:
F. Warranty Documentation: Submit manufacturer’s standard warranty.2
. A.B.53) . Product Data: Submit manufacturer’s product data. REFERENCE STANDARDS
Specifier Notes: List reference standards mentioned in this section. and date of application. B. Comply with Section 01330 (01 33 00) – Submittal Procedures. B. This article does not require compliance with reference standards. Manufacturer’s Project References: Submit manufacturer’s list of successfully completed concrete tennis court surface color coating system projects.
Specifier Notes: Submit independent test results for solar reflectance index to qualify for LEED credits. Samples: Submit manufacturer’s color samples of color coating.
02790 (32 18 23. including project name. Delete reference standards not included in this edited section. Applicator’s Project References: Submit applicator’s list of successfully completed concrete tennis court surface color coating system projects. 1.4
Specifier Notes: Edit submittal requirements as required. D. and date of application. location. complete with designations and titles. E. United States Tennis Association (USTA) Rules of Tennis.
2 A.53) . for past 5 years. 5. Crack Sealant: SportMaster “Crack Magic”.
MANUFACTURER SportMaster Sport Surfaces. AMBIENT CONDITIONS Do not apply concrete tennis court surface color coating system when air or surface temperatures are below 50 degrees F during application or within 24 hours after application. MATERIALS Concrete Tennis Court Surface Color Coating System: SportMaster Color Coating System. dry area indoors. Toll Free 800-326-1994. and application to prevent contamination or damage.1. Member: ASBA.
PART 2 2. AND HANDLING Delivery and Acceptance Requirements: Deliver materials to site in manufacturer’s original. 3.6 A. Keep materials from freezing. Applicator regularly engaged. with labels clearly identifying product name and manufacturer. 2. Store and handle materials in accordance with manufacturer’s instructions.
2. 4. unopened containers and packaging. 2. Sandusky.sportmaster.net. DELIVERY.
1. 3. Store materials in clean. Protect materials during storage.net. 2. in manufacture of asphalt tennis court surface color coating systems of similar type to that specified. in application of tennis court surface color coating systems of similar type to that specified. 100 percent acrylic emulsion elastomeric crack sealant. PO Box 2277.
B. Keep materials in manufacturer’s original. Do not apply concrete tennis court surface color coating system when rain is expected during application or within 24 hours after application.
Applicator's Qualifications: 1. B.7 A. 6. 2520 South Campbell Street.3
Manufacturer regularly engaged. handling. for past 3 years.
B. Employ persons trained for application of tennis court surface color coating systems. Store materials out of direct sunlight. Storage and Handling Requirements: 1.
02790 (32 18 23. Fax 877-825-9226. unopened containers and packaging until application. B. 7. Website www. E-mail info@sportmaster. Close containers when not in use. United States owned company. Ohio 44870. STORAGE.1 A. PRODUCTS
5 lbs. c.0 percent.
F.0 percent.5 lbs.5 percent. plus or minus 5 percent. Additives: 1. Mineral Inert Fillers: 78. Minimum: a. 4. plus or minus 0. plus or minus 0.
E.2 percent. Mix on-site with silica sand. Levels and repairs low spots and depressions up to 3/4 inch deep in concrete pavement.0 lbs. Hiding Pigment: 2. 7. 2. 2. 4. d.4
.5 percent.8 percent. 2.7 lbs. Weight per Gallon at 77 Degrees F: 8. Non-Volatile Material: 80 percent. Weight per Gallon at 77 Degrees F: 8. 6. Acrylic Emulsion: 10.
02790 (32 18 23. Chemical Characteristics.2 percent.. Film Formers.8 lbs.0 percent. 3. Mix on-site with sand and cement.
Specifier Notes: Specify color of filler course.8 lbs. Non-Volatile Material: 27. 1. 100 percent acrylic emulsion trowel-grade crack filler.0 percent. D. C. plus or minus 0. Adhesion Promoter: SportMaster “Acrylic Adhesion Promoter”. 4.
Patch Binder: SportMaster “Acrylic Patch Binder”. Water: 45... 5. 3.0 percent. Weight per Gallon at 77 Degrees F: 15. 3.. Filler Course: SportMaster “Acrylic Resurfacer”.2 lbs. Minimum: a. 100 percent acrylic emulsion liquid binder. Color: [Green] [Neutral] [Red]. 5.2. Color: [Black] [Neutral]. Acrylic emulsion primer.53) .0 percent. by Weight. Additives: 0. 3. by Weight.5 lbs. Weight per Gallon at 77 Degrees F: 8. 1. 4. e. Mineral Inert Fillers: 5. plus or minus 0. c.
Crack Filler: SportMaster “Acrylic Crack Patch”. Acrylic Emulsion: 44. Primes concrete surface and promotes adhesion of color coating system materials. Non-Volatile Material: 61 percent. Hiding Pigment: 0.5 lbs.. Fills cracks in concrete pavement up to 1 inch wide. 6. Chemical Characteristics. Weight per Gallon at 77 Degrees F: 8. e. b.5 lbs. Film Formers. 3. plus or minus 5 percent. plus or minus 5.0 percent. 1.
Specifier Notes: Specify color of crack filler. Water: 8. 2. 100 percent acrylic emulsion resurfacer. plus or minus 1. d. Apply to adhesion promoter or previously colored acrylic surfaces in preparation of color coating system.
Seals cracks up to 1/2 inch wide in concrete pavement. 1. b.
Pigmented.12 percent. d.1 A.1: Heat Island Effect – Non-Roof: Dove Gray. Light Green. Additives: 1. Pigment: 14. plus or minus 5 percent. Hiding Pigment: 0. and Sandstone.
H. Weight per Gallon at 77 Degrees F: 8.0 percent. Line marking on concrete tennis courts. Water: 50.9 lbs. 100 percent acrylic emulsion coating. The following colors can contribute to LEED credits for SS Credit 7.53) .90 percent.0 percent. Water: 41. Color: [Blue] [Red] [White] [Yellow].5 lbs.2 lbs. Acrylic Emulsion: 38. 4. Weight per Gallon at 77 Degrees F: 10. Additives: 4. b. Color: [Beige] [Blue] [Brown] [Dark Green] [Dove Gray] [Forest Green] [Gray] [Ice Blue] [Light Blue] [Light Green] [Maroon] [Red] [Sandstone] [Tournament Purple]. clear drying.0 percent.G. d.. by Weight. 3. c. 5.65 lbs. 5. 5. 3. by Weight. 100 percent acrylic emulsion primer.
02790 (32 18 23.89 percent. Nominal: a. 6. Primes line markings and prevents bleed-under for sharp lines. PART 3 3. Acrylic Emulsion: 25.0 percent. Film Formers.
I. Non-Volatile Material: 29 percent.73 percent. Nominal: a. c.5
. e. Weight per Gallon at 77 Degrees F: 9. 3. 2.36 percent. Chemical Characteristics. 1. Mineral Inert Fillers: 13. EXECUTION
EXAMINATION Examine concrete tennis court surfaces to receive color coating system. Chemical Characteristics.
Specifier Notes: Specify color of color coating.
Color Coating: SportMaster “ColorPlus System”. 1.5 percent. Red.75 lbs. 2. 100 percent acrylic emulsion line paint.5 lbs. 1. Line Paint: SportMaster “Textured Line Paint”. Color coats tennis courts. plus or minus 0.. Mineral Inert Fillers: 7. 4. e. b.
Line Markings Primer: SportMaster “Stripe-Rite”.17 percent. Non-Volatile Material: 45. 2. 4. plus or minus 5 percent.
Specifier Notes: Specify color of line paint. plus or minus 0. plus or minus 0.. Ice Blue. Mix on-site with silica sand and water.
3. then rinse thoroughly.
E. 3. Prepare surfaces in accordance with manufacturer’s instructions.2 A. Existing Concrete: 1. 2. Remove dirt. Notify Architect of conditions that would adversely affect application or subsequent use. shotblast. D. H.53) .
C. Sandblast. vegetation. or scarify smooth concrete surfaces to roughened texture similar to medium broom finish. APPLICATION Apply concrete tennis court surface color coating system in accordance with manufacturer’s instructions at locations indicated on the Drawings. Provide medium broom finish or similar roughened texture. Apply adhesion promoter over entire concrete surface in accordance with manufacturer’s instructions. Do not steel trowel finish.B. Repair spalled areas and level depressions 1/8 inch and deeper with patch binder in accordance with manufacturer’s instructions. loose coatings. J.
02790 (32 18 23. New Concrete: 1. Acid etch surface per manufacturers specifications. 2. Ensure surface repairs are flush and smooth to adjoining surfaces. debris.
G. Apply 1 coat of filler course to provide smooth underlayment for application of color coating. Perimeter drainage to prevent moisture accumulation beneath concrete surface. oil. depressions. 3. Cure new concrete surfaces a minimum of 28 days before application of concrete tennis court surface color coating system.
Verify: 1. C. 3.6
D. 4. and other surface contaminants which could adversely affect application of concrete tennis court surface color coating system. grease. 2.
B. Acid etch surface per manufacturers specifications. SURFACE PREPARATION Protection of In-Place Conditions: Protect adjacent surfaces and landscaping from contact with concrete tennis court surface color coating system. Repair cracks. Do not begin surface preparation or application until unacceptable conditions are corrected. curing compounds. Suitable vapor barrier beneath concrete slab.3 A. Pressure wash entire surface. dust. and surface defects in accordance with manufacturer’s instructions before application of color coating. Concrete tennis courts meet ASBA requirements. sealers.
I. loose materials. then rinse thoroughly.
E. Filler Course: 1. F.
Mix materials in accordance with manufacturer’s instructions. C. Apply a minimum of 1 coat of line paint in accordance with manufacturer’s instructions.4 A. 3. Apply Filler Course and Color Coating with a 50-60 durometer. LINE MARKINGS Lay out tennis court line markings in accordance with USTA Rules of Tennis. 3. Apply 2 coats on existing acrylic surfaces with extensive cracks or low spot repair.
02790 (32 18 23. to seal voids between masking tape and tennis court surface to prevent bleed-under when line paint is applied. B. Apply line markings primer. soft rubber squeegee.7
.53) . Apply 1 coat on new concrete or existing acrylic surfaces with minimal repairs. Protect applied concrete tennis court surface color coating system to ensure that. coating system will be without damage or deterioration at time of Substantial Completion.B. D. 2. Allow material drying times in accordance with manufacturer’s instructions before applying other materials or opening completed surface to foot traffic.5 A. after masking tape has been laid. B. C. except for normal weathering. PROTECTION Allow a minimum of 24 hours curing time before opening tennis courts for play. Apply a minimum of 2 coats of color coating to prepared surfaces in accordance with manufacturer’s instructions.
Documents Similar To SportMaster Concrete Tennis Court Surface Color Coating System - Guide SpecificationCPSkip carouselThe Artist in YouArtistsNetwork_AcrylicPainting_2016Plastiment®PR650sAntisol S.pdfm.tech Structures AnalysisSika® ViscoCrete®-4100MCI-2246[1]1296810722477-ch05Sika Solutions for Waste Water Treatment Plants LowK38L_ENG_0610 Mobilna Pumpa CifaComparative Statement for Apcbtmp WorksBasf MasterGlenium ACE 8381 Tds18 WP Concrete Coating 18Design Criteria Final Draft (5!08!09)ConcreteIS:4926 RMCManual Respinse 2000FinalPune Universityppi_091985SeminarsConplast NcA Method for Mix-Design of Fiber-reinforced Self-compacting ConcreteConcreteConcreting-Method Statement OriginalB35 TANIM.pdfPenstock CodeNalsr NotesIES Civil Engineering Paper 1 2003M.tech(Structural)SyllabusDocuments About Acrylic PaintSkip carouselHenry Schein Brand CatalogArt at the Capitol bookletAcrylic WallsUT Dallas Syllabus for arts3366.001.11s taught by Lorraine Tady (ltt042000)UT Dallas Syllabus for arts3369.001.10f taught by Lorraine Tady (ltt042000)UT Dallas Syllabus for arts3369.001.11s taught by Lorraine Tady (ltt042000)UT Dallas Syllabus for arts3369.001.11f taught by Lorraine Tady (ltt042000)UT Dallas Syllabus for arts3366.001.11f taught by Lorraine Tady (ltt042000)More From insane88Skip carouselSoil Bearing Capacity and Modulus of Subgrade ReactionPenetron_Admix_Brochure.pdfA Steel ShopsGoogle వార్తలుGoogle NewsTecheBusiness & FinancialHalloween Prank TraditionAutraliaInternacionalwired newsIndia.pdf102412pdf24World Economy RealityTop GearScienceEgypt AirMicrosoft CorporationSouth China SeaTrumpRandomsTera DataKuala Lumpur, Federal Territory of..TechnologyHealthWorldWorldSciencePeak Ground Acceleration - Wikipedia, The Free Encyclopedia